LMucko/crystallography-open-database huggingface dataset:
Neutron diffraction study of stoichiometric spinel Li1+x Mn2-x O4 showing octahedral 16c-site Li-occupation
Berg, H.; Kelder, E. M.; Thomas, J. O.; Journal of Materials Chemistry 9 (1999) 427–429; doi:10.1039/a804851g

data_7214216
_publ_section_title
;
 Neutron diffraction study of stoichiometric spinel Li1+x Mn2-x O4 showing
 octahedral 16c-site Li-occupation
;
_journal_coden_ASTM              JMACEP
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              427
_journal_page_last               429
_journal_paper_doi               10.1039/a804851g
_journal_volume                  9
_journal_year                    1999
_chemical_formula_structural     'Li1.14 Mn1.86 O4'
_chemical_formula_sum            'Li1.14 Mn1.86 O4'
_chemical_name_systematic
;
Lithium Manganese Oxide (1.14/1.86/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2001/07/16
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.1784(6)
_cell_length_b                   8.1784(6)
_cell_length_c                   8.1784(6)
_cell_volume                     547.02(7)
_refine_ls_R_factor_all          0.054
_cod_data_source_file            'data_LiMn2O4melanie088469.cif'
_cod_data_source_block           1395826945.29-D290F29E9218B844.cif
_cod_original_cell_volume        547.02
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               7214216
Neutron and X-ray powder diffraction studies of Li Mn2-y Cry O4
Oikawa, K.; Kamiyama, T.; Izumi, F.; Nakazato, D.; Ikuta, H.; Wakihara, M.; Journal of Solid State Chemistry 146 (1999) 322–328; doi:10.1006/jssc.1999.8351

data_1513996
_publ_section_title
;
 Neutron and X-ray powder diffraction studies of Li Mn2-y Cry O4
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              322
_journal_page_last               328
_journal_paper_doi               10.1006/jssc.1999.8351
_journal_volume                  146
_journal_year                    1999
_chemical_formula_structural     'Li Mn2 O4'
_chemical_formula_sum            'Li Mn2 O4'
_chemical_name_systematic
;
Lithium Manganese(III) Manganese(IV) Oxide
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2001/07/16
_audit_update_record             2008/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.24376(13)
_cell_length_b                   8.24376(14)
_cell_length_c                   8.24376(14)
_cell_volume                     560.242(16)
_refine_ls_R_factor_all          0.025
_cod_data_source_file            'data_LiMn2O4melanie088644.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395827069.56-D290F29E9218B844.cif
_cod_original_cell_volume        560.24
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'Li1 Mn2 O4'
_cod_database_code               1513996
Neutron diffraction study of electrochemically delithiated Li Mn2 O4 spinel
Berg, H.; Thomas, J. O.; Solid State Ionics 123 (1999) 227–234; doi:

data_1513997
_publ_section_title
;
 Neutron diffraction study of electrochemically delithiated Li Mn2 O4
 spinel
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              227
_journal_page_last               234
_journal_volume                  123
_journal_year                    1999
_chemical_formula_structural     'Li Mn2 O4'
_chemical_formula_sum            'Li Mn2 O4'
_chemical_name_systematic
;
Lithium Manganese(III) Manganese(IV) Oxide
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2002/04/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.2211(4)
_cell_length_b                   8.2211(4)
_cell_length_c                   8.2211(4)
_cell_volume                     555.64(5)
_refine_ls_R_factor_all          0.045
_cod_data_source_file            'data_LiMn2O4melanie089459.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395827154.13-D290F29E9218B844.cif
_cod_original_cell_volume        555.64
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'Li1 Mn2 O4'
_cod_database_code               1513997
Neutron diffraction study of electrochemically delithiated Li Mn2 O4 spinel
Berg, H.; Thomas, J. O.; Solid State Ionics 123 (1999) 227–234; doi:

data_1513999
_publ_section_title
;
 Neutron diffraction study of electrochemically delithiated Li Mn2 O4
 spinel
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              227
_journal_page_last               234
_journal_volume                  123
_journal_year                    1999
_chemical_formula_structural     'Li0.74 Mn2 O4'
_chemical_formula_sum            'Li0.74 Mn2 O4'
_chemical_name_systematic        'Lithium Manganese Oxide (0.74/2/4)'
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2002/04/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.144(2)
_cell_length_b                   8.144(2)
_cell_length_c                   8.144(2)
_cell_volume                     540.1(2)
_refine_ls_R_factor_all          0.015
_cod_data_source_file            'data_LiMn2O4melanie089460.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395827235.74-D290F29E9218B844.cif
_cod_original_cell_volume        540.15
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               1513999
Neutron diffraction study of electrochemically delithiated Li Mn2 O4 spinel
Berg, H.; Thomas, J. O.; Solid State Ionics 123 (1999) 227–234; doi:

data_1514001
_publ_section_title
;
 Neutron diffraction study of electrochemically delithiated Li Mn2 O4
 spinel
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              227
_journal_page_last               234
_journal_volume                  123
_journal_year                    1999
_chemical_formula_structural     'Li0.28 Mn2 O4'
_chemical_formula_sum            'Li0.28 Mn2 O4'
_chemical_name_systematic        'Lithium Manganese Oxide (0.28/2/4)'
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2002/04/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.043(1)
_cell_length_b                   8.043(1)
_cell_length_c                   8.043(1)
_cell_volume                     520.30(11)
_refine_ls_R_factor_all          0.016
_cod_data_source_file            'data_LiMn2O4melanie089461.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395827370.62-D290F29E9218B844.cif
_cod_original_cell_volume        520.3
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               1514001
Zur Kenntnis von Oxyden A (M O4): Ueber Li Mn O4, K Mn O4, Rb Mn O4, Cs Mn O4 sowie Rb I O4 und Cs I O4. (-Was heisst eigentlich "Die Kristallstruktur von..."?-)
Hoppe, R.; Fischer, D.; Schneider, J.; Zeitschrift fuer Anorganische und Allgemeine Chemie 625 (1999) 1135–1142; doi:10.1002/(SICI)1521-3749(199907)625:7<1135::AID-ZAAC1135>3.0.CO;2-L

data_1514003
_publ_section_title
;
 Zur Kenntnis von Oxyden A (M O4): Ueber Li Mn O4, K Mn O4, Rb Mn O4, Cs
 Mn O4 sowie Rb I O4 und Cs I O4. (-Was heisst eigentlich "Die
 Kristallstruktur von..."?-)
;
_journal_coden_ASTM              ZAACAB
_journal_name_full
;
 Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              1135
_journal_page_last               1142
_journal_paper_doi
10.1002/(SICI)1521-3749(199907)625:7<1135::AID-ZAAC1135>3.0.CO;2-L
_journal_volume                  625
_journal_year                    1999
_chemical_formula_structural     'Li (Mn O4)'
_chemical_formula_sum            'Li Mn O4'
_chemical_name_systematic        'Lithium Manganate(VII)'
_space_group_IT_number           63
_symmetry_Int_Tables_number      63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_audit_creation_date             2002/04/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            4
_cell_length_a                   5.51402(8)
_cell_length_b                   8.39754(15)
_cell_length_c                   6.35911(10)
_cell_volume                     294.454(8)
_refine_ls_R_factor_all          0.021
_cod_data_source_file            'data_LiMnO4melanie089505.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395827583.97-D290F29E9218B844.cif
_cod_original_cell_volume        294.45
_cod_original_formula_sum        'Li1 Mn1 O4'
_cod_database_code               1514003
Single crystal X-ray diffraction study of the spinel-type LiMn~2~O~4~
Akimoto, Junji; Takahashi, Yasuhiko; Gotoh, Yoshito; Mizuta, Susumu; Chemistry of Materials 12 (2000) 3246–3248; doi:10.1021/cm0003673

data_4001896
_publ_section_title
;
 Single crystal X-ray diffraction study of the spinel-type LiMn~2~O~4~
;
_journal_coden_ASTM              CMATEX
_journal_issue                   11
_journal_name_full               'Chemistry of Materials'
_journal_page_first              3246
_journal_page_last               3248
_journal_paper_doi               10.1021/cm0003673
_journal_volume                  12
_journal_year                    2000
_chemical_formula_structural     'Li Mn2 O4'
_chemical_formula_sum            'Li Mn2 O4'
_chemical_name_systematic        'Lithium Manganese(III) Manganese(IV) Oxide'
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2002/04/01
_audit_update_record             2008/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.2483(6)
_cell_length_b                   8.2483(6)
_cell_length_c                   8.2483(6)
_cell_volume                     561.17(7)
_refine_ls_R_factor_all          0.024
_cod_data_source_file            'data_LiMn2O4melanie089985.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395827659.85-D290F29E9218B844.cif
_cod_original_cell_volume        561.17
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'Li1 Mn2 O4'
_cod_database_code               4001896
Relationship of crystal structure to interionic interactions in the lithium-manganese spinel oxides
Piszora, P.; Catlow, C. R. A.; Woodley, S. M.; Wolska, E.; Computers and Chemistry 24 (2000) 609–613; doi:

data_1514004
_publ_section_title
;
 Relationship of crystal structure to interionic interactions in the
 lithium-manganese spinel oxides
;
_journal_coden_ASTM              COCHDK
_journal_name_full               'Computers and Chemistry'
_journal_page_first              609
_journal_page_last               613
_journal_volume                  24
_journal_year                    2000
_chemical_formula_structural     '(Li0.956 Mn0.044) Mn2 O4'
_chemical_formula_sum            'Li0.956 Mn2.044 O4'
_chemical_name_systematic
;
Lithium Manganese Oxide (0.96/2.04/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_audit_creation_date             2002/04/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.2579(3)
_cell_length_b                   8.2579(3)
_cell_length_c                   8.2579(3)
_cell_volume                     563.13(4)
_refine_ls_R_factor_all          0.047
_cod_data_source_file            'data_LiMn2O4melanie090131.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395831526.71-D290F29E9218B844.cif
_cod_original_cell_volume        563.13
_cod_original_sg_symbol_H-M      'F d -3 m S'
_cod_database_code               1514004
Relationship of crystal structure to interionic interactions in the lithium-manganese spinel oxides
Piszora, P.; Catlow, C. R. A.; Woodley, S. M.; Wolska, E.; Computers and Chemistry 24 (2000) 609–613; doi:

data_1514005
_publ_section_title
;
 Relationship of crystal structure to interionic interactions in the
 lithium-manganese spinel oxides
;
_journal_coden_ASTM              COCHDK
_journal_name_full               'Computers and Chemistry'
_journal_page_first              609
_journal_page_last               613
_journal_volume                  24
_journal_year                    2000
_chemical_formula_structural
;
(Li0.989 Mn0.011) (Li0.060 Mn1.940) O4
;
_chemical_formula_sum            'Li1.049 Mn1.951 O4'
_chemical_name_systematic
;
Lithium Manganese Oxide (1.05/1.95/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_audit_creation_date             2002/04/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.1845(3)
_cell_length_b                   8.1845(3)
_cell_length_c                   8.1845(3)
_cell_volume                     548.25(3)
_refine_ls_R_factor_all          0.05
_cod_data_source_file            'data_LiMn2O4melanie090132.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395831594.53-D290F29E9218B844.cif
_cod_original_cell_volume        548.25
_cod_original_sg_symbol_H-M      'F d -3 m S'
_cod_database_code               1514005
Syntheses, structures, and preliminary electrochemistry of the layered lithium and sodium manganese(IV) oxides, A~2~Mn~3~O~7~
Raekelboom, E.; Hector, A. L.; Owen, J.; Vitins, G.; Weller, M. T.; Chemistry of Materials 13 (2001) 4618–4623; doi:10.1021/cm011105j

data_4001897
_publ_section_title
;
 Syntheses, structures, and preliminary electrochemistry of the layered
 lithium and sodium manganese(IV) oxides, A~2~Mn~3~O~7~
;
_journal_coden_ASTM              CMATEX
_journal_issue                   12
_journal_name_full               'Chemistry of Materials'
_journal_page_first              4618
_journal_page_last               4623
_journal_paper_doi               10.1021/cm011105j
_journal_volume                  13
_journal_year                    2001
_chemical_formula_structural     'Li0.48 (Mn0.89 O2)'
_chemical_formula_sum            'Li0.48 Mn0.89 O2'
_chemical_name_systematic        'Lithium Manganese Oxide (0.48/0.89/2)'
_space_group_IT_number           166
_symmetry_Int_Tables_number      166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_audit_creation_date             2003/04/01
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   2.83961(11)
_cell_length_b                   2.83961(11)
_cell_length_c                   14.486(5)
_cell_volume                     101.16(4)
_refine_ls_R_factor_all          0.047
_cod_data_source_file            'data_LiMnO2melanie092859.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395831734.17-D290F29E9218B844.cif
_cod_original_cell_volume        101.16
_cod_original_sg_symbol_H-M      'R -3 m H'
_cod_database_code               4001897
Single crystal growth of the spinel-type Li Mn2 O4
Akimoto, J.; Takahashi, Y.; Gotoh, Y.; Mizuta, S.; Journal of Crystal Growth 229 (2001) 405–408; doi:10.1016/S0022-0248(01)01190-3

data_1514006
_publ_section_title
;
 Single crystal growth of the spinel-type Li Mn2 O4
;
_journal_coden_ASTM              JCRGAE
_journal_name_full               'Journal of Crystal Growth'
_journal_page_first              405
_journal_page_last               408
_journal_paper_doi               10.1016/S0022-0248(01)01190-3
_journal_volume                  229
_journal_year                    2001
_chemical_formula_structural     'Li Mn2 O4'
_chemical_formula_sum            'Li Mn2 O4'
_chemical_name_systematic
;
Lithium Manganese(III) Manganese(IV) Oxide
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2003/04/01
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.2483(6)
_cell_length_b                   8.2483(6)
_cell_length_c                   8.2483(6)
_cell_volume                     561.17(7)
_cod_data_source_file            'data_LiMn2O4melanie093599.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395831853.52-D290F29E9218B844.cif
_cod_original_cell_volume        561.17
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'Li1 Mn2 O4'
_cod_database_code               1514006
Topotactic reactions, structural studies and lithium intercalation in cation-deficient spinels with formula close to Li2 Mn4 O9
Ibarra Palos, A.; Anne, M.; Strobel, P.; Journal of Solid State Chemistry 160 (2001) 108–117; doi:10.1006/jssc.2001.9200

data_1514007
_publ_section_title
;
 Topotactic reactions, structural studies and lithium intercalation in
 cation-deficient spinels with formula close to Li2 Mn4 O9
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              108
_journal_page_last               117
_journal_paper_doi               10.1006/jssc.2001.9200
_journal_volume                  160
_journal_year                    2001
_chemical_formula_structural     'Li0.78 Mn1.88 O4'
_chemical_formula_sum            'Li0.78 Mn1.88 O4'
_chemical_name_mineral           Unnamed_Spinel
_chemical_name_systematic
;
Lithium Manganese Oxide (0.78/1.88/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2003/04/01
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.1811(3)
_cell_length_b                   8.1811(3)
_cell_length_c                   8.1811(3)
_cell_volume                     547.56(3)
_refine_ls_R_factor_all          0.016
_cod_data_source_file            'data_LiMn2O4melanie093742.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395831952.55-D290F29E9218B844.cif
_cod_original_cell_volume        547.56
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               1514007
The Li Mn2 O4 to lambda-(Mn O2) phase transition studied by in situ neutron diffraction
Berg, H.; Rundlof, H.; Thomas, J. O.; Solid State Ionics 144 (2001) 65–69; doi:10.1016/S0167-2738(01)00894-3

data_1514008
_publ_section_title
;
 The Li Mn2 O4 to lambda-(Mn O2) phase transition studied by in situ
 neutron diffraction
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              65
_journal_page_last               69
_journal_paper_doi               10.1016/S0167-2738(01)00894-3
_journal_volume                  144
_journal_year                    2001
_chemical_formula_structural     'Li Mn2 O4'
_chemical_formula_sum            'Li Mn2 O4'
_chemical_name_systematic
;
Lithium Manganese(III) Manganese(IV) Oxide
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2003/10/01
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.225(1)
_cell_length_b                   8.225(1)
_cell_length_c                   8.225(1)
_cell_volume                     556.43(12)
_refine_ls_R_factor_all          0.0194
_cod_data_source_file            'data_LiMn2O4melanie094339.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395832086.33-D290F29E9218B844.cif
_cod_original_cell_volume        556.43
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'Li1 Mn2 O4'
_cod_database_code               1514008
The Li Mn2 O4 to lambda-(Mn O2) phase transition studied by in situ neutron diffraction
Berg, H.; Rundlof, H.; Thomas, J. O.; Solid State Ionics 144 (2001) 65–69; doi:10.1016/S0167-2738(01)00894-3

data_1514009
_publ_section_title
;
 The Li Mn2 O4 to lambda-(Mn O2) phase transition studied by in situ
 neutron diffraction
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              65
_journal_page_last               69
_journal_paper_doi               10.1016/S0167-2738(01)00894-3
_journal_volume                  144
_journal_year                    2001
_chemical_formula_structural     'Li Mn2 O4'
_chemical_formula_sum            'Li Mn2 O4'
_chemical_name_systematic
;
Lithium Manganese(III) Manganese(IV) Oxide
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2003/10/01
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.206(1)
_cell_length_b                   8.206(1)
_cell_length_c                   8.206(1)
_cell_volume                     552.58(12)
_refine_ls_R_factor_all          0.0156
_cod_data_source_file            'data_LiMn2O4melanie094340.cif'
_cod_data_source_block
/var/www/cod/tmp/uploads/1395832161.4-D290F29E9218B844.cif
_cod_original_cell_volume        552.58
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'Li1 Mn2 O4'
_cod_database_code               1514009